ARTICLESPUBLISHED ONLINE: 28 SEPTEMBER 2015 | DOI: 10.1038/NMAT4425
Plasmons in graphene moiré superlatticesG. X. Ni1,2, H.Wang3, J. S. Wu2, Z. Fei2, M. D. Goldflam2, F. Keilmann4, B. Özyilmaz1, A. H. Castro Neto1,X. M. Xie3, M. M. Fogler2 and D. N. Basov2*
Moiré patterns are periodic superlattice structures that appear when two crystals with a minor lattice mismatch aresuperimposed. A prominent recent example is that of monolayer graphene placed on a crystal of hexagonal boron nitride.As a result of the moiré pattern superlattice created by this stacking, the electronic band structure of graphene is radicallyaltered, acquiring satellite sub-Dirac cones at the superlattice zone boundaries. To probe the dynamical response of the moirégraphene, we use infrared (IR) nano-imaging to explore propagation of surface plasmons, collective oscillations of electronscoupled to IR light. We show that interband transitions associated with the superlattice mini-bands in concert with freeelectrons in the Dirac bands produce two additive contributions to composite IR plasmons in graphene moiré superstructures.This novel form of collective modes is likely to be generic to other forms of moiré-forming superlattices, including van derWaals heterostructures.
The interaction of the nearly matching hexagonal lattices ofgraphene and hexagonal boron nitride (hBN) results in aquasiperiodic moiré superlattice1–3. The consequences are
marked: a new set of superlattice Dirac mini-bands emerges ingraphene/hBN heterostructures, leading to a rich variety of interest-ing effects4–10. Evidence for the superlattice mini-bands is found inboth spectroscopic and transport measurements1,6,11–14. The opticalconductivity4,15 and the plasmon dispersion15 in moiré graphenehave been investigated theoretically. An intriguing prediction15 isthat an additional low-frequency plasmon branch may exist in arange of Fermi energies where the partially gapped mini-bandscontain small pockets of carriers that are split off from the Diracbands. However, no experimental study of plasmonic phenomenain moiré-patterned graphene (MPG) has yet been reported. Thequest to fully examine these phenomena is exacerbated by the small(sub-µm2) area of typical superlattice domains that often occur inthe immediate proximity of plain graphene (Fig. 1). To alleviatethis problem, we made use of the propagating surface plasmonpolariton waves launched in the setting of scattering-type scanningnear-field optical microscopy (s-SNOM) measurements, therebyenabling experimental access to the electronic band structure andelectron–hole excitations of the nanoscalemoiré-patterned domainsin graphene. Our analysis of plasmonic real-space fringes revealsthat bound electrons in the superlattice mini-bands create novelcollective characteristics in moiré graphene.
We have carried out nano-IR imaging of Dirac plasmons atUCSD by means of the s-SNOM apparatus (Fig. 1a; see Methods).In this instrument a metallized tip (antenna) of an atomic forcemicroscope (AFM) with curvature radius ∼25 nm was illuminatedby IR light, generating strong enhancement of the electric fieldunderneath the tip. This antenna-based nano-IR set-up circumventsthe momentum mismatch between light and surface plasmons ingraphene16, allowing us to launch plasmonic waves of wavelengthλp. These waves propagate radially outwards from the tip and formplasmon fringes with a period of λp/2 owing to the interference be-tween tip-launched and edge-reflected plasmonwaves16,17. Together,
the wavelength of the plasmonic fringes, the rate at which plasmonicoscillations decay in the interior of the sample, and the amplitude ofthe overall nano-IR scattering signal contain complete informationon the complex conductivity of the graphene layer at the frequencyof the IR probe beam ω.
Our graphene microcrystals were grown by means of catalyst-free epitaxial synthesis on top of hBN/quartz18–20 (see Methods).The key advantage of this synthesis approach over the commonlyused dry transfer method1,11–14 is that graphene microcrystals canbe naturally aligned with respect to the hBN lattice, forming MPGwith a wavelength λµ∼14 nm (Fig. 1b,c). Moreover, our approachyields high-quality graphene flakes free of the polymer residuals,bubbles or wrinkles that often plague structures fabricated usingalternative methods.
In Fig. 1d, we show typical nano-IR imaging data. Here we plotraster-scanned images of the normalized back scattering amplitudesignal s(ω) at a selected IR frequency ω= 890 cm−1. The MPGregions are directly adjacent to plain (free of superlattice effects)graphene: a virtue that has allowed us to examine the impact ofthe moiré superlattice in the same microcrystal. These two adjacentregions of a single microcrystal share an identical environment,assuring that the carrier density (n) due to the unintentionaldoping is uniform through the entire microcrystal21,22. The mostprominent aspect of the images in Fig. 1d is that the magnitudeof the scattering amplitude in MPG regions is enhanced relativeto plain graphene (Fig. 1e). Furthermore, every boundary of thesample in Fig. 1d prompts periodic oscillations of the nano-IRsignal. These oscillations are signatures of plasmonic reflections thatoccur at sample edges and at the borders of regions with differentcomplex conductivity σ(ω)= σ1(ω)+ iσ2(ω) (ref. 23). Therefore,the observed plasmonic reflections are consistent with the notionof dissimilar values of σ(ω) in MPG and plain graphene.
The nano-IR data in Fig. 1d give a rich insight into the electronicprocesses in moiré superlattices that ultimately govern plasmonpropagation and reflection in this system. It is therefore instructiveto closely examine the line-profiles along the direction normal to
1Centre for Advanced 2DMaterials and Graphene Research Centre, National University of Singapore, Singapore 117546, Singapore. 2Department ofPhysics, University of California, San Diego, La Jolla, California 92093, USA. 3State Key Laboratory of Functional Materials for Informatics, ShanghaiInstitute of Microsystem and Information Technology, Chinese Academy of Sciences, 865 Changning Road, Shanghai 200050, China.4Ludwig-Maximilians-Universität and Center for Nanoscience, 80539 München, Germany. *e-mail: [email protected]
Figure 1 | AFM and plasmon nano-imaging with s-SNOM. a, Schematic of the nano-IR imaging set-up. b, AFM topography image of a G/hBN sample withboth a moiré-patterned (regime 1) and a non-patterned regime (regime 2). Regime 3 corresponds to the bare hBN. c, A higher-resolution image(friction-AFM) at the boundary between the moiré-patterned and plain graphene, as marked by the dashed square in b. The superstructure in regime 1exhibits hexagonal symmetry with lattice constant λµ∼ 14 nm; whereas regime 2 shows no noticeable variation. d, Nano-IR images of the normalizedscattering amplitude s(ω) as introduced in the text. Scale bars, 1 µm (b,d); 40 nm (c). e, Line-profile across the boundary between MPG and plain grapheneindicated in d. The profiles are averaged over a width of 100 nm.
the sample edges of both MPG and plain graphene for sampleswith a range of carrier concentrations. In Fig. 2 we show tracesobtained by averaging 102 such line-profiles from each sample.These data capture the salient trends in the evolution of theplasmonic response, both in the MPG and plain graphene regions,with variation of the carrier density. Even though our structuresare not gate-tunable, by exploring a large number of samples withdifferent levels of unintentional doping, we were able to grasp thepertinent effects of carrier density variation. The half-wavelength ofthe plasmons in Fig. 2 can be approximately determined from thefull-width at half-maximum of the dominant fringe; this protocolis validated through numerical modelling, which captures thegross features of the plasmonic line-profiles (see SupplementaryInformation). This analysis revealed that plasmons in the MPGand plain graphene regions in the same microcrystal are of similarwavelengths. The data series in Fig. 2 shows that the plasmonwavelength for plain graphene varies between approximately 50 nmand 220 nm. The plasmon wavelength is given by λp=2π/q1, whereq1 is the real part of the complex plasmon wavenumber qp =q1+ iq2. The latter is related to the complex conductivity σ(ω) ofgraphene via16:
where the effective permittivity of the substrate εsub is the geometricmean of the in- and out-of-plane permittivities24. In plain graphenewe can approximate σ(ω) using the common Drude model,
τ−1− iω, D=
πh̄2 EF (2)
which has two parameters: Drude weight D and relaxation time τ .Combining equations (1) and (2), one finds the well-known linearscaling between λp and the Fermi energy EF:
h̄2ω2[1+εsub(ω)], EF= h̄vF
On the basis of equation (3), we conclude that the variation ofthe carrier density for data in Fig. 2a–f is from n= 8× 1011 cm−2to n= 8.5× 1012 cm−2. For the plain graphene, the gross trendsin Fig. 2 repeat the behaviour of gated structures16,17,25. At allcarrier densities, the dominant fringe (closest to the sample edge)is present, with additional higher-order fringes appearing in theprofiles, corresponding to higher carrier densities. For the smallestand largest carrier densities (Fig. 2a,f), both the MPG regions andplain graphene show nearly matching line-profiles. In contrast toplain graphene, in the intermediate doping regime, the line-profilesfor MPG areas do not reveal additional, weaker fringes (panels inFig. 2c–e). Instead, in this regime, MPG samples show an overallincrease of the scattering amplitude in the interior of the samples,without additional fringe structure.
We now proceed to quantitatively analyse the trends seen inMPG and plain graphene. First, we will extract the complexconductivity of graphene from the raw line-profile data (symbols inFig. 3a,b). Then we will compare these results with the conductivitycalculated theoretically for plain and moiré superlattice graphene.The line-profiles in Fig. 2 are uniquely determined by the complexmomentum of the plasmon qp, which, according to equation (1), isdirectly related to the conductivity of graphene. In Fig. 3a,b we showthe conductivity extracted from fitting of plasmonic line-profiles(see Supplementary Information). In the case of plain graphene, theconductivity and the magnitude of EF are expected to be linearlyrelated according to equation (2). This dependence is obeyed in ourplain graphene samples (Fig. 3a). As for the MPG, the connectionbetween the conductivity and the Fermi energy must be evaluatednumerically (Supplementary Information). In contrast to the linearchange seen in plain graphene, a nonlinear variation of the realpart of the conductivity σ1(ω= 890 cm−1) with EF in MPG can beseen in Fig. 3b. Another quantity of interest is the damping factorγp ∼σ1/σ2 (Fig. 3c). In plain graphene the magnitude of γp is nearlyindependent of EF, whereas in MPG we observe a non-monotonicvariation of damping with EF, with a broadmaximum at EF∼ 0.2 eV.
We wish to point out that in addition to the damping causedby the inter-mini-band transitions specific to the superlattice(see below), loss mechanisms present in plain graphene (impurities,
Figure 2 | Plasmonic line-profiles for both moiré-patterned graphene(MPG) and plain graphene (PG) at di�erent carrier densities. These datawere collected for specimens with di�erent levels of unintentional dopingas marked in the frame. From a to f, the corresponding plasmon wavelengthλp increases from 50nm to 220 nm, as described in the text. The grapheneis to the right of the shaded region.
electron–electron, electron–phonon interaction) are most certainlypresent in MPG. Such contributions are likely to be additive, atleast, when each of them is weak. Recent calculations of plasmondamping due to electron scattering by impurities26, other electrons27and acoustic phonons24,25 identified the latter as the dominantdissipationmechanism in high-mobility graphene at ambient. Thesecalculations predict that the relaxation rate, τ−1(ω), varies withfrequency, which explains why using the transport time from thed.c. conductivity underestimates the plasmon damping at mid-IR frequencies25. Our model of plasmon damping, which uses anadjustable and ω-independent parameter τ , is still oversimplified.As moiré graphene is a much more complicated system thanplain graphene, a diagrammatic calculation of electron–phonon
0.1 0.2 0.3 0.4
0.1 0.2 0.3 0.4
PG (exp.)MPG (model)
0.1 0.2 0.3 0.4
2 (exp.)σ1 (model)σ
2 (exp.)σ1 (model)σ
Figure 3 | Extraction of optical conductivity and plasmon damping.a,b, The red and black data points are the optical conductivity from plaingraphene (a) and MPG (b) extracted from the imaging data atω=890 cm−1 as a function of Fermi energy EF. The red and black dashedlines are the modelling results for both σ1 and σ2 at room temperature.c, The red and black data points are the extracted plasmon damping γpplotted as a function of EF from the MPG and plain graphene, respectively.The experimental values of γp were obtained from the ratio of σ1 and σ2.The open triangles for EF∼0.1 eV data points signify a larger uncertainty offitting at low carrier density. The red and black dashed lines are themodelling results of the plasmon damping rate for both MPG and plaingraphene, respectively. The error bars represent the 95%confidence intervals.
scattering24 is challenging. However imperfect our modellingapproach is, it does highlight stark distinctions in the plasmondamping between plain graphene and MPG.
To determine the origin of themeasured variation of the complexconductivity of MPG, we consider optical transitions (Fig. 4b,c)enabled by the moiré superlattices, which we computed following
Figure 4 | Electronic band structure and the optical conductivity of graphene moiré superlattices. a, 3D representation of the electronic band structure ofMPG obtained from the phenomenological model as described in the Supplementary Information. The impact of the superlattice modulation is moreprominent for the hole side than for the electron side. b,c, Band structure for MPG presented in the superlattice zone scheme for two di�erent positions ofthe Fermi level. b, For a magnitude of the EF smaller than Eµ, the moiré potential causes additional optical transitions once the carrier densitynmin∼6.3× 1011 cm−2 is reached. c, For a magnitude of EF larger than Eµ one finds multiple additional channels for optical transitions, all initiated by themoiré potential. These transitions enhance the conductivity and also yield an interband contribution to the plasmonic wavelength in addition to intrabandcontribution due to the Dirac cones at the γ points. d, Theoretical conductivity spectra σ1(ω) calculated for MPG at di�erent values of EF in thelow-temperature conditions. The dashed green curve represents σ1(ω) for plain graphene at EF=−210meV for comparison. Inset shows the product ofσ2(ω)ω for MPG at di�erent magnitudes of EF. The dashed green curve represents σ2(ω)ω for plain graphene at EF=−210meV for comparison.e, Calculated 2D mapping of σ1 as a function of ω and EF. The dashed line indicates the experimental probing frequency of 890 cm−1. The circled numbers1,2,3 in c–e represent the superlattice mini-band resonances.
previous studies3,4,6,15, as detailed in Supplementary Section III. Themoiré potential introduces several important energy scales, suchas Eµ= gνF/2≈ 170meV, where νF is the Fermi velocity of plaingraphene and g=2π/λµ is the superlattice momentum. This energyscale is roughly equal to the electron energy at the µ-points of themini Brillouin zone (Fig. 4a–c). It defines characteristic featuresof the particle–hole excitations of MPG that can be recognizedin the spectra of the optical conductivity (Fig. 4d,e). Specifically,at ω= 2Eµ, the σ1(ω) spectra acquire a weak structure owing totransitions between the µ-points of the conduction and valencebands6. Furthermore, in doped (or gated) MPG specimens, therelationship between Eµ and EF defines characteristic attributes ofthe optical conductivity in the following three regimes: |EF|�Eµ,|EF|'Eµ, |EF|>Eµ all relevant to the range of carrier densities in thedata set shown in Figs 2 and 3.
In weakly dopedMPG (|EF|�Eµ), the conductivity is dominatedby the low-energy regions of the electron spectra, preserving theirDirac-like character even in the superlattice samples. For simplicity,we assumed here that MPG is incommensurate and has no gap
at the Dirac point6,10,12. In this regime, the dominant feature ofthe conductivity spectra is the onset of transitions between thetwo linearly dispersing mini-bands (the blue bands in Fig. 4a–c).This step-like onset is seen at ω= 1,100 cm−1 in the red trace ofFig. 4d (EF=−70meV) and as the sharp change near the diagonalof the false colour conductivity map in Fig. 4e, where ω= 2EF.The interband spectral weight missing below 2EF reappears in theintraband transitions (Drude peak) atω=0 (refs 28,29). Apart fromthe weak features at 2Eµ, the conductivities of the plain and weaklydoped MPG almost coincide. Accordingly, imaging data in Fig. 2areveal nearly identical plasmonic patterns.
As doping increases and the magnitude of EF approaches Eµ,transitions involving another pair ofmini-bands (the blue and eitherthe green or the red valence bands in Fig. 4a–c) become significant.The details of themini-band absorption depend on the assumptionsfor the potentials describing the interaction of graphene with hBN.One possible outcome is the formation of gapless mini-bands withreplicas of Dirac cones. Alternatively, some or all of mini-bandsmayacquire the energy gaps (Fig. 4b,c): a scenario that most accurately
NATUREMATERIALS DOI: 10.1038/NMAT4425 ARTICLESreproduces the totality of experimental data in Figs 2 and 3, aswill be detailed below. Within this latter scenario, the transitionsalong γ–µ and along γ–κ and γ–κ′ produce threshold features atωmin≈ 2Eµ− 2EF (Fig. 4b) and ω≈[(
respectively. These transitions prompt a pair of the descendingdiagonal lines in Fig. 4e. Along the µ–κ path, the dispersions ofthe green and blue valence bands are almost parallel (nested),being separated by ∆µ–κ≈ 380 cm−1, as indicated in Fig. 4c. Sucha nesting is responsible for the strong resonance at ω≈∆µ–κ inthe conductivity spectra when EF falls within ∼∆µ–κ from −Eµ(the blue trace in Fig. 4d and the leftmost ‘hot region’ in Fig. 4e).The ∆µ–κ-resonance is directly relevant to the plasmonic imagingdata in Fig. 2b–d because its influence remains appreciable at ourprobing frequency of 890 cm−1. This resonance both enhances theoverall contrast due to MPG and suppresses weaker (higher-order)plasmonic fringes in these data. At higher EF two other interbandresonances appear (the magenta trace in Fig. 4d and the othertwo ‘hot regions’ in Fig. 4e). These are due to the approximatenesting of the green and red valence bands along the γ–κ(∆γ–κ≈200 cm−1) and γ–κ′(∆γ–κ′≈690 cm−1) paths in Fig. 4c. (Forthe chosen simulation parameters themagnitudes of∆µ–κ,∆γ–κ and∆γ–κ′ already deviate by ∼20% from the lowest-order perturbativeformulae3.) Overall, the gapped mini-band contribution to σ1(ω)spectra at the frequency of our plasmonic probe is peaked atthe doping level corresponding to EF ∼ 0.2 eV and is slightlyreduced at higher doping. In contrast, gapless mini-bands lead to amonotonic variation of the conductivity with EF (see SupplementaryInformation). We therefore conclude that a model of gapped mini-bands is fully consistent with the findings of plasmonic imaging.
To describe the caveats of the measured plasmon wavelength inMPG at appreciable doping levels |EF|> Eµ, we now turn to theanalysis of the product σ2(ω)ω. These spectra help to illustrate theredistribution of the spectral weight between inter- and intra-mini-band transitions in MPG. In the limit of ω→0 this product yields30the spectral weight of a narrow Drude peak σ2(ω)ω≈D, that in thecase of plain graphene is given by equation (2). As expected, in plaingraphene the product σ2(ω)ω is approximately constant in the rangeτ−1�ω�2EF (Fig. 4d, inset). However, inMPG the low-frequencybehaviour of σ2(ω)ω is more complicated because of additionalinter-mini-band transitions. At τ 1
�ω�min(∆µ–κ,∆γ–κ,∆γ–κ′),the product σ2(ω)ω yields the intra-mini-band part of the spectralweight. As exemplified by the spectrum for EF =−210meV, themagnitude of this Drude-like weight is reduced15 compared to thatof the plain graphene of the same Fermi energy, equation (2). Asfrequency increases, the product σ2(ω)ω reveals a minimum in thevicinity of ω=580 cm−1, and thereafter plateaus at the same level asin the plain graphene (see the dashed curve in Fig. 4d, inset). Thenet result is that the magnitude of σ2(ω) at frequencies far abovethe inter-mini-band resonances, ω�∆=max(∆µ–κ,∆γ–κ,∆γ–κ′),is the same in plain graphene and MPG, as demanded by theoscillator strength sum rule31,32. Hence, we arrive at the notion ofa composite plasmon in moiré superlattices originating from thetwo additive contributions: the usual Drude channel (that is, of theungapped portion of the Fermi surface) and the interband channelassociated with the superlattice mini-bands (the gapped portion ofthe Fermi surface). In our data collected at ambient, the differencesof response of plain graphene and MPG is masked by finitetemperature effects, as T = 300K corresponds to approximately∆/3.We anticipatemore prominent near-field contrast and strongerplasmonic reflections at the boundary of plain and moiré grapheneat lower T and/or lower frequencies ω < ∆ (see below andSupplementary Information).
We now wish to outline some implications of our work andsome problems for future study. First, we have shown that theinterface of plain graphene and MPG acts as a plasmonic reflectorwith a doping-dependent reflection coefficient (Supplementary
Information). This implies that plasmonic reflectors formed at theboundary between MPG and plain graphene can also be tunedwith the single gate voltage applied to the entire structure, whichmay be advantageous for implementation of graphene plasmoniccircuits33. These tunable metasurfaces are a prerequisite for theimplementation of transformation plasmonics34, which offers thecapability to control plasmonic fields at will and allow novelfunctionalities that were not previously attainable (SupplementaryInformation). Second, a more complete experimental picture of theelectromagnetic response of the moiré graphene may be obtainedby extending our approach to terahertz and far-IR regions wherethe composite plasmon is predicted to generate an additional low-energy plasmon branch (see ref. 15 and Supplementary Fig. 7).The recent development of alternative broadband light sources,such as synchrotron light or free-electron lasers, opens thedoor towards nano-imaging experiments at far-IR frequencies35–40.Finally, in our model, graphene is assumed to be perfectly rigid andincommensurate with the hBN. It will be worthwhile investigatingif plasmonic spectroscopy can reveal subtle topological effects thatarise from deformation of the graphene lattice and the inducedlattice commensurability12.
MethodsMethods and any associated references are available in the onlineversion of the paper.
Received 6 April 2015; accepted 17 August 2015;published online 28 September 2015
References1. Dean, C. R. et al.Hofstadter’s butterfly and the fractal quantum Hall effect in
moiré superlattices. Nature 497, 598–602 (2013).2. Xue, J. et al. Scanning tunnelling microscopy and spectroscopy of ultra-flat
graphene on hexagonal boron nitride. Nature Mater. 10, 282–285 (2011).3. Wallbank, J. R., Patel, A. A., Mucha-Kruczyński, M., Geim, A. K. & Fal’ko, V. I.
Generic miniband structure of graphene on a hexagonal substrate. Phys. Rev. B87, 245408 (2013).
4. Abergel, D. S. L., Wallbank, J. R., Chen, X., Mucha-Kruczyński, M. &Fal’ko, V. I. Infrared absorption by graphene-hBN heterostructures. New J.Phys. 15, 123009 (2013).
5. Basov, D. N., Fogler, M. M., Lanzara, A., Wang, F. & Zhang, Y. Colloquium:Graphene spectroscopy. Rev. Mod. Phys. 86, 959–993 (2014).
6. Shi, Z. et al. Gate-dependent pseudospin mixing in graphene/boron nitridemoiré superlattices. Nature Phys. 10, 743–747 (2014).
7. Yankowitz, M., Xue, J. & LeRoy, B. J. Graphene on hexagonal boron nitride.J. Phys. Condens. Matter 26, 303201 (2014).
8. Gorbachev, R. V. et al. Detecting topological currents in graphene superlattices.Science 346, 448–451 (2014).
9. San-Jose, P., Gutiérrez-Rubio, A., Sturla, M. & Guinea, F. Electronic structure ofspontaneously strained graphene on hexagonal boron nitride. Phys. Rev. B 90,115152 (2014).
10. Chen, Z. G. et al. Observation of an intrinsic bandgap and Landau levelrenormalization in graphene/boron-nitride heterostructures. Nature Commun.5, 4461 (2014).
11. Yu, G. L. et al.Hierarchy of Hofstadter states and replica quantum Hallferromagnetism in graphene superlattices. Nature Phys. 10, 525–529 (2014).
12. Woods, C. R. et al. Commensurate–incommensurate transition in graphene onhexagonal boron nitride. Nature Phys. 10, 451–456 (2014).
13. Hunt, B. et al.Massive Dirac fermions and Hofstadter butterfly in a van derWaals heterostructure. Science 340, 1427–1430 (2013).
14. Ponomarenko, L. A. et al. Cloning of Dirac fermions in graphene superlattices.Nature 497, 594–597 (2013).
15. Tomadin, A., Guinea, F. & Polini, M. Generation and morphing of plasmons ingraphene superlattices. Phys. Rev. B 90, 161406(R) (2014).
16. Fei, Z. et al. Gate-tuning of graphene plasmons revealed by infrarednano-imaging. Nature 487, 82–85 (2012).
17. Chen, J. et al.Optical nano-imaging of gate-tunable graphene plasmons. Nature487, 77–81 (2012).
18. Tang, S. et al. Precisely aligned graphene grown on hexagonal boron nitride bycatalyst free chemical vapor deposition. Sci. Rep. 3, 2666 (2013).
19. Tang, S. et al. Silane-catalysed fast growth of large single-crystalline grapheneon hexagonal boron nitride. Nature Commun. 6, 6499 (2015).
36. Hermann, P. et al. Characterization of semiconductor materials usingsynchrotron radiation-based near-field infrared microscopy and nano-FTIRspectroscopy. Opt. Express 22, 17948–17958 (2014).
37. Fehrenbacher, M. et al. Plasmonic superlensing in doped GaAs. Nano Lett. 15,1057–1061 (2015).
38. Hegenbarth, R. et al.High-power femtosecond mid-IR sources for s-SNOMapplications. J. Opt. 16, 094003 (2014).
39. Bensmann, S. et al. Near-field imaging and spectroscopy of locally strainedGaN using an IR broadband laser. Opt. Express 22, 22369–22381 (2014).
40. Huber, A. J., Keilmann, F., Wittborn, J., Aizpurua, J. & Hillenbrand, R.Terahertz near-field nanoscopy of mobile carriers in single semiconductornanodevices. Nano Lett. 8, 3766–3770 (2008).
AcknowledgementsWork at the University of California, San Diego (UCSD), on optical phenomena in vdWmaterials is supported by DOE-BES DE-FG02-00ER45799. Research at UCSD on tunableplasmonic reflectors is supported by ONR. D.N.B. is funded by the Gordon andBetty Moore Foundation’s EPiQS Initiative through Grant GBMF4533. The developmentof scanning plasmon interferometry is supported by DOE-BES and ARO. G.X.N., B.Ö.and A.H.C.N. acknowledge the National Research Foundation, Prime Minister Office,Singapore, under its Medium Sized Centre Program and CRP award ‘Novel 2D materialswith tailored properties: beyond graphene’ (R-144-000-295-281).
Author contributionsAll authors were involved in designing the research, performing the research, and writingthe paper.
Additional informationSupplementary information is available in the online version of the paper. Reprints andpermissions information is available online at www.nature.com/reprints.Correspondence and requests for materials should be addressed to D.N.B.
Competing financial interestsF.K. is one of the co-founders of Neaspec, producer of the s-SNOM apparatus used inthis study.
NATUREMATERIALS DOI: 10.1038/NMAT4425 ARTICLESMethodsHexagonal boron nitride (hBN) flakes were prepared on quartz substrates usingmechanical exfoliation. Graphene microcrystals were then epitaxially grownon top of hBN using a catalysis-free chemical vapour deposition (CVD; ref. 18).First, the hBN flakes on quartz were annealed at 1,150 ◦C at low pressure with acontinuous argon flow of 50 standard cubic centimetres per minute (sccm) for30min. Then, graphene was grown on the hBN flakes at 1,150 ◦C by flowingCH4:H2 at 5:5 sccm for 300min at pressures below 12mbar. After growth,samples were cooled to room temperature in argon flow. The morphology, grainsize, shape and crystallographic orientation of the CVD graphene can be controlledby varying growth conditions. Clusters of polycrystalline graphene are oftendetected in samples grown at a lower temperature. In macroscopic samplesprepared using catalyst-free synthesis, MPG (λµ∼14 nm, θ∼0◦) regionscommonly reside next to plain graphene (λµ<0.5 nm, θ∼30◦): a virtue that
allowed us to examine the impact of the moiré superlattice in the sameparticular microcrystals.
The infrared nano-imaging experiments were performed using ascattering-type scanning near-field optical microscope (s-SNOM). Our s-SNOM(http://www.neaspec.com) is equipped with continuous-wave mid-IR quantumcascade lasers (http://www.daylightsolutions.com) and CO2 lasers(http://www.accesslaser.com). The s-SNOM is based on an atomic forcemicroscope (AFM) operating in the tapping mode with a tapping frequencyaround 270 kHz. A pseudo-heterodyne interferometric detection module isimplemented in our s-SNOM to extract both the scattering amplitude s and phaseψ of the near-field signal. In the current work, we discuss the amplitude of thesignal. To subtract the background signal, we demodulated the near-field signal atthe third harmonic of the tapping frequency. All the infrared nano-imagingexperiments were performed in ambient conditions.